LMucko/crystallography-open-database huggingface dataset:
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 1st run, T = 400 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007197
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 1st run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1263
_cell_length_b                   8.1263
_cell_length_c                   8.1263
_cell_formula_units_Z            8
_cell_volume                     536.634
_database_code_amcsd             0008782
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.605
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007197
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 1st run, T = 450 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007198
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 1st run, T = 450 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1305
_cell_length_b                   8.1305
_cell_length_c                   8.1305
_cell_formula_units_Z            8
_cell_volume                     537.467
_database_code_amcsd             0008783
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    3.600
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007198
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 1st run, T = 400 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007199
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 1st run, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1265
_cell_length_b                   8.1265
_cell_length_c                   8.1265
_cell_formula_units_Z            8
_cell_volume                     536.674
_database_code_amcsd             0008784
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.605
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007199
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 1st run, T = 28 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007200
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 1st run, T = 28 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1018
_cell_length_b                   8.1018
_cell_length_c                   8.1018
_cell_formula_units_Z            8
_cell_volume                     531.795
_database_code_amcsd             0008785
_diffrn_ambient_temperature      301.15
_exptl_crystal_density_diffrn    3.638
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007200
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 2nd run, T = 500 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007201
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 2nd run, T = 500 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1338
_cell_length_b                   8.1338
_cell_length_c                   8.1338
_cell_formula_units_Z            8
_cell_volume                     538.122
_database_code_amcsd             0008786
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.595
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007201
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 2nd run, T = 450 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007202
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 2nd run, T = 450 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1302
_cell_length_b                   8.1302
_cell_length_c                   8.1302
_cell_formula_units_Z            8
_cell_volume                     537.407
_database_code_amcsd             0008787
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    3.600
_cod_original_cell_volume        537.408
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007202
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 550 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007203
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 550 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1379
_cell_length_b                   8.1379
_cell_length_c                   8.1379
_cell_formula_units_Z            8
_cell_volume                     538.936
_database_code_amcsd             0008788
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    3.590
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007203
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 600 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007204
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1419
_cell_length_b                   8.1419
_cell_length_c                   8.1419
_cell_formula_units_Z            8
_cell_volume                     539.731
_database_code_amcsd             0008789
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.585
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007204
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 650 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007205
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 650 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1461
_cell_length_b                   8.1461
_cell_length_c                   8.1461
_cell_formula_units_Z            8
_cell_volume                     540.567
_database_code_amcsd             0008790
_diffrn_ambient_temperature      923.15
_exptl_crystal_density_diffrn    3.579
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007205
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 700 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007206
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1502
_cell_length_b                   8.1502
_cell_length_c                   8.1502
_cell_formula_units_Z            8
_cell_volume                     541.383
_database_code_amcsd             0008791
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.574
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007206
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 800 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007207
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1577
_cell_length_b                   8.1577
_cell_length_c                   8.1577
_cell_formula_units_Z            8
_cell_volume                     542.879
_database_code_amcsd             0008792
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.564
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007207
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 900 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007208
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 900 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1658
_cell_length_b                   8.1658
_cell_length_c                   8.1658
_cell_formula_units_Z            8
_cell_volume                     544.498
_database_code_amcsd             0008793
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.553
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007208
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: M-Cr, 3rd run, T = 1000 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007209
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: M-Cr, 3rd run, T = 1000 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.868 Cr0.123 Mg0.999 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1733
_cell_length_b                   8.1733
_cell_length_c                   8.1733
_cell_formula_units_Z            8
_cell_volume                     546.000
_database_code_amcsd             0008794
_diffrn_ambient_temperature      1273.15
_exptl_crystal_density_diffrn    3.544
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.868 Mg.999 Cr.123 Mn.002 Zn.007 O4'
_cod_database_code               9007209
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 25 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007210
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1080
_cell_length_b                   8.1080
_cell_length_c                   8.1080
_cell_formula_units_Z            8
_cell_volume                     533.017
_database_code_amcsd             0008795
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.655
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007210
How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high temperature in natural spinels Sample: H-Cr, 1st run, T = 200 C
Martignago, F.; Dal Negro, A.; Carbonin, S.; Physics and Chemistry of Minerals 30 (2003) 401–408; doi:10.1007/s00269-003-0336-0

data_9007211
_publ_section_title
;How Cr3+ and Fe3+ affect Mg-Al order-disorder transformation at high
 temperature in natural spinels Sample: H-Cr, 1st run, T = 200 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              401
_journal_page_last               408
_journal_paper_doi               10.1007/s00269-003-0336-0
_journal_volume                  30
_journal_year                    2003
_chemical_formula_sum            'Al1.834 Cr0.162 Mg0.995 Mn0.002 O4 Zn0.007'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1180
_cell_length_b                   8.1180
_cell_length_c                   8.1180
_cell_formula_units_Z            8
_cell_volume                     534.992
_database_code_amcsd             0008796
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    3.642
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.834 Mg.995 Cr.162 Mn.002 Zn.007 O4'
_cod_database_code               9007211